POWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS


 Leon Summers
 2 years ago
 Views:
Transcription
1 EXPERIMENT 4 POWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS I. Introduction The determination of the chemical structure of molecules is indispensable to chemists in their effort to gain insight into chemical problems. Only a few physical methods are capable of determining chemical structure, and amongst these methods, diffraction methods have been the most successful. Diffraction methods are capable of defining bond lengths, bond angles and the spatial proximity of nonbonded atoms for materials capable of forming crystalline solids. For example, the models of myoglobin which were displayed in the fluoridemyoglobin lab are representations of the myoglobin structure found using xray diffraction. The importance of structural determination to science has been recognized with several Nobel Prizes for xray diffraction related research. Year Prize Awardee Topic 1914 Physics M. Von Laue Discovery of xray diffraction 1915 Physics W.H. Bragg Analysis of crystal structure using xray W.L. Bragg diffraction 1962 Chemistry J.C. Kendrew M.F. Perutz Structural determination of globular proteins (myoglobin and hemoglobin) 1964 Chemistry D.C. Hodgkin Structure determinations of important biochemical molecules 1962 Medicine F.H. Crick Structure of DNA J.D. Watson M.H. Wilkins 199? Chemistry J. Deisenhofer R. Huber H. Michel Structure of photosynthetic reaction center In this final laboratory exercise, you will determine the structure and unit cell dimension of an alkali halide crystal using powder xray diffraction, and use the data to construct a chart of ionic radii.
2 To explain xray diffraction it is convenient to think of light as a wave with a wavelength that is related to the energy of the light by the equation, E=hc/λ, where h is Plank s constant, c is the speed of light and λ is the wavelength of light. For light within the xray region of the spectrum, the wavelength of the light is within the range 0.1Å to 100Å. One of the fundamental properties of waves is that two waves can interfere with each other if they are in the same spatial region. If the phases of the two waves are coincident they will constructively interfere (increased amplitude) and if their phases are opposed they will destructively interfere (decreased amplitude). Constructive Interference Destructive Interference Wave 1 Wave 2 Sum 1+2 Wave 1 Wave 2 Sum 1+2 The interference patterns formed in xray diffraction originates from the xrays that are scattered by the electrons of atoms within a crystalline solid. A simple picture of a solid (composed of only one type of atom) is a collection of balls packed together to form a crystal lattice. In a crystalline material the packing of the atoms is well defined, and in fact, the entire crystal can be constructed by repeating a pattern of atoms that define the unit cell (see Chang, chapter 11, Kotz, chapter 13). This is analogous to the fact that a wall can be constructed by stacking bricks; the brick is the unit cell of the wall. The simplest case (the only one that we will consider) is when the unit cell is cubic, that is to say that all of the edges of the cube are equal and the corners form right angles. For cubic unit cells the length of the edge is usually given the symbol a. Due to the regular spacing of the atoms, imaginary planes can be pictured which contain the nuclei. For example, each face of the cube in the illustration above is one such plane. The electrons of each of these imaginary planes of atoms scatter the xrays giving a result that can be interpreted as set of parallel partial mirrors; the light (xrays) is partially reflected by each plane. Although the xrays originate inphase from the xray source, the scattered xrays are not necessarily in phase when they emerge from the crystal and reach the detector. The relative phases of scattered x rays depend critically on the separation distance between these imaginary planes. This is due to the fact that xrays that penetrate deeper into the 2 Larsen 4:20 Spring 2000
3 crystal lattice before they are reflected, travel further. Simple geometry demonstrates that for two waves reflected by adjacent planes, the wave that is reflected by the second plane has traveled a distance of (2d sinθ) further than the wave that is reflected by the first plane. In general, the reflected waves from successive planes destructively interfere, however, if the pathlength difference between reflected waves is an integer multiple of the wavelength (λ), constructive interference is observed (a bright spot). This condition (the Bragg s condition for constructive interference) is summarized by Bragg s Law: nλ = 2d sinθ, where λ is the wavelength, d is the interplanar separation, and θ is the Bragg s angle. The n defines the order of the reflection, with n=1 giving firstorder, n=2 giving secondorder, etc. From the above equation, it is evident that the structure of the solid (i.e. the distance between the atoms) can be obtained if a monochromatic xray source is used (only one λ) and the intensity of xrays is measured as a function of θ. The constructive interference that results at specific values of theta (θ) map out the interplanar spacing of the solid. Further, the total intensity at a spot, not only depends on the fulfillment of the Bragg s condition, but also on the number of electrons, which depends on the chemical identity of the atoms. There is one further complication however, the planes of atoms can be constructed in several different ways as illustrated below. Each imaginary plane can be indexed using Miller indices. The Miller index is written as three numbers, (h k l), one for each coordinate in three dimensional space. The protocol for writing these indices are given in the reference 1, but for now just consider them as labeling scheme for all possible imaginary planes. Each plane can satisfy the Bragg s condition and give a bright spot due to constructive interference. To account for all possible planes, the Bragg s Law is usually rewritten (for a cubic system) as, ( ) sin 2 λ 2 θ = 4a 2 h 2 + k 2 + l 2 1 Start at the origin of the unit cell, then determine where the point where the plane intersects each of the three axes (a,b,c) of the cell. (abc is used for crystal coordinate rather than xyz) If a plane is parallel to an axis it is assigned an intercept of infinity ( ). The Miller index is form by dividing the cell dimension along each axis (a,b,c), by the intercept to general the Miller indices (h,k,l) respectively. For example, if the intersection occur half way alone a then h=a/(a/2)=2. 3 Larsen 4:20 Spring 2000
4 where a is the unit cell dimension, λ is the wavelength of the radiation, (h, k, l) are the Miller indices, and θ is the Bragg angle. In a powder, composed of a very large number of crystallites, all possible orientations of the crystal are simultaneously present. This means that the Bragg s condition for constructive interference will be fulfilled simultaneously for all possible planes consistent with the given crystalline structure. Therefore, a diffraction pattern, intensity as a function of the scattering angle (2θ), is generated and is directly related to the arrangement of atoms within the unit cell as well as to the distances between the atoms. As you will recall from 4:14 or 4:19 (see Chang, chapter 11, Kotz, chapter 13), ionic solids composed of alkali halides tend to form cubic crystals with either an FCC (face centered cubic) or simple cubic (primative) unit cell. 2 In this laboratory exercise, you will determine the unit cell structure and unit cell dimension of a series of alkali halide salts. By using the cumulative data of the series you will also determine the cation and anion radii in the lattice. To acquire the data needed to determine these radii, you will use the Chemistry Department s powder xray diffractometer (powder XRD) which was purchased in 1996 for ~$130,000 (needless to say, each student will not have her/his own instrument). II. Experimental (groups of four) The sample preparation and data acquisition for this lab are almost trivial. Each group member will be responsible for one sample from the following set of alkali halides: NaF, NaCl, NaBr, NaI, KCl, KBr, and CsCl. In addition, a powder diffraction pattern of LiCl, will be provided to each group. Each group member should begin her/his numerical analysis on the LiCl data. Experimental diffraction patterns will be obtained for each of the other samples. The sample preparation consists of grinding the sample in a mortar and pestle and placing a 2 There is one other variant of the cubic unit cell known as BCC (body centered cubic), but the alkali halides do not crystallize with this structure. 4 Larsen 4:20 Spring 2000
5 flattened pile of salt on a glass plate. The plate is then placed into the sample holder and a diffraction pattern is obtained using the wavelength of Å (CuK α, isolated with a Ni foil filter). Your TA or safety monitor will help you will this step. The data will be printed as intensity as a function of scattering angle (2Θ). Each set of reflections will be analyzed to determine the structure (primitive or FCC) and the unit cell dimension. For the simple cubic unit cells, all possible combinations of integer Miller indices are possible. In general for FCC, certain combinations of Miller indices are eliminated by destructive interference caused by the planes formed by the atoms in the faces of the unit cell. The result is that for FCC type lattices reflections occur only if h, k, and l are all even or all odd. There is one caveat though, in FCC systems in which the scattering power of the two types of atoms is nearly identical (i.e. when the two ions have the same number of electrons) a pseudoprimitive pattern (one that looks primitive) is observed; this is the case for KCl. These results can be used to assign the diffraction patterns and extract the lattice type and cell dimensions from the data. Simple Cubic (h k l) Body Centered Cubic (h k l) Face Centered Cubic (h k l) h 2 + k 2 + l , To correlate the observed Bragg s angle with the predicted values the data must be manipulated to resemble the Bragg s law, sin 2 θ = λ2 4a 2 h 2 + k 2 + l 2. This is most easily accomplished using a spreadsheet program such as KaleidaGraph or Excel. First, enter the position of each reflection and label the column 2theta. Construct a second column that equals sin 2 θ. This is c1=(sin(c0/2))^2 in KaleidaGraph (or =SIN(PI()*A2/360)^2 in Excel then fill down). Realize that Bragg s law has the form sin 2 θ=c*i, where C is a constant equal to λ 2 C = 4a 2 and i is an integer as indicated in the table above. Therefore, divide the experimental values of sin 2 θ by the sin 2 θ value of the first reflection (c2=c1/ sin 2 θ reflection1 ). If the unit cell is simple cubic, the result of this operation should give an integer series starting with one (see table above). If the unit cell is FCC, the column will need to be multiplied by 3 before the expected integer series is obtained. (There will be some experimental error). Once the unit cell type has been established create a column that contains the expected integer values for the appropriate cell type (e.g. 3,4,8,11,12 for FCC). 5 Larsen 4:20 Spring 2000
6 Graph sin 2 θ vs. the integer column (y vs. x) and fit the result to a straight line to obtain the constant, C. λ 2 Use the wavelength of λ= Å to solve for the constant, a using C = 4a 2. To determine if the constant, a, represents the unit cell dimension, half of the unit cell dimension, or twice the unit cell dimension, requires that the density calculated from the cell volume be compared to the actual (macroscopic) density. The simple cubic unit cell contains 1 molecule (AX) and the FCC contains 4 molecules (4 AX). The volume is the cell length cubed, and density is mass divided by volume. The experimental values for density as well as cell parameter data (for comparison to your own) is presented in the table below. You will find that in the case of KCl and CsI the unit cell may need to be contracted or expanded (why are these special cases?). Salt a o (Å) Density (g/cm 3 ) Molecular Weight (g/mol) Lattice Type NaF Ca FCC LiCl FCC NaCl FCC KCl FCC (pseudosimple) CsCl Simple Cubic NaBr FCC KBr FCC CsI Simple Cubic (pseudobodycentered) Data from F.P. Boer, and T.H. Jordan, J. Chem. Educ., 42, 76 (1965). Ionic radii will be calculated following the seminal work of Landé, 3 which was one of the first determinations of the values for ionic radii. Landé assumed that due to the small size of the lithium cation, the unit cell dimension of lithium halides was determined by anion anion contacts. By inspection of the FCC unit cell, four times the radius of the halide atom is seen to be 4r Cl = 2a o. Once this value is set, r=1.81å in the case of Cl, other radii can be obtained by assuming that cationanion contacts determine the edge length. Again inspection of the unit cell leads to the conclusion that: a o = 2r cation + 2r anion in the case of FCC and 3a o =2r cation + 2r anion in the case of simple cubic. (Br , 1.96Å; Na +, 1.01Å; K +, 1.34Å; and Cs +, 1.76Å) 3 A. Landé, Z. Physik, 1, 191 (1920). 6 Larsen 4:20 Spring 2000
7 Prelab Questions (15 points) Answer these questions in your laboratory notebook. 1. Go to the Nobel prize web site at the URL, For one of the Nobel prizes mentioned in this handout, read any one of the following: presentation/speech, press release or a bibliography of one of the scientist. Write a oneparagraph summary of the historic event or person. (10 points) 2. To obtain the powder diffraction patterns of the alkali halides you will use xrays of wavelength λ=1.54å. The diffraction pattern will be a plot of xray intensity vs. the scattering angle, 2Θ. To better see what is going on, go to the Bragg s Law and Diffraction simulation at: Enter a wavelength of λ=1.54å. Choose on salt: NaF, CsCl, or CsI. Use the table in this handout to the unit cell dimension.(e.g. LiCl is a o =5.13Å, do not use this salt, ). Enter the cell dimension into the simulation. Now enter 5 for the beginning angle. Click on the box that says, details. Use the greater than sign (>) to scan the angle. Record the values of theta that give maximum constructive interference and the value of theta that give maximum destructive interference over the range theta=5 to 35. Mathematically determine the value of theta that gives the first order scattering condition for the salt that you used in the simulation. (5 points) No purpose or procedure is needed for the prelab this week. Lab Report (35 points) Your lab report should be completed in your laboratory notebook. Hand in the original to your TA. The laboratory report for this lab will consist of all the required calculations, and a brief summary of your results. The report will be turned in at the end of section. There will also be a short exercise that to determine the line spacing of a diffraction pattern that will also be completed while in the laboratory. 7 Larsen 4:20 Spring 2000
Crystal Structure Determination I
Crystal Structure Determination I Dr. Falak Sher Pakistan Institute of Engineering and Applied Sciences National Workshop on Crystal Structure Determination using Powder XRD, organized by the Khwarzimic
More informationThe Crystal Structures of Solids
The Crystal Structures of Solids Crystals of pure substances can be analyzed using Xray diffraction methods to provide valuable information. The type and strength of intramolecular forces, density, molar
More informationXRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US. Hanno zur Loye
XRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye Xrays are electromagnetic radiation of wavelength about 1 Å (1010 m), which is about the same size as an atom. The
More informationChapter 3. 1. 3 types of materials amorphous, crystalline, and polycrystalline. 5. Same as #3 for the ceramic and diamond crystal structures.
Chapter Highlights: Notes: 1. types of materials amorphous, crystalline, and polycrystalline.. Understand the meaning of crystallinity, which refers to a regular lattice based on a repeating unit cell..
More informationStructure Factors 59553 78
78 Structure Factors Until now, we have only typically considered reflections arising from planes in a hypothetical lattice containing one atom in the asymmetric unit. In practice we will generally deal
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationBCM 6200  Protein crystallography  I. Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS
BCM 6200  Protein crystallography  I Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS Elastic Xray Scattering From classical electrodynamics, the electric field of the electromagnetic
More informationCrystal Structure of High Temperature Superconductors. Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson
Crystal Structure of High Temperature Superconductors Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson Introduction History of Superconductors Superconductors are material which
More informationChem 106 Thursday Feb. 3, 2011
Chem 106 Thursday Feb. 3, 2011 Chapter 13: The Chemistry of Solids Phase Diagrams  (no BornHaber cycle) 2/3/2011 1 Approx surface area (Å 2 ) 253 258 Which C 5 H 12 alkane do you think has the highest
More informationXray Diffraction and EBSD
Xray Diffraction and EBSD Jonathan Cowen Swagelok Center for the Surface Analysis of Materials Case School of Engineering Case Western Reserve University October 27, 2014 Outline Xray Diffraction (XRD)
More informationChapter 7: Basics of Xray Diffraction
Providing Solutions To Your Diffraction Needs. Chapter 7: Basics of Xray Diffraction Scintag has prepared this section for use by customers and authorized personnel. The information contained herein is
More informationIntroduction to Powder XRay Diffraction History Basic Principles
Introduction to Powder XRay Diffraction History Basic Principles Folie.1 History: Wilhelm Conrad Röntgen Wilhelm Conrad Röntgen discovered 1895 the Xrays. 1901 he was honoured by the Noble prize for
More informationXRay Diffraction. wavelength Electric field of light
Light is composed of electromagnetic radiation with an electric component that modulates versus time perpendicular to the direction it is travelling (the magnetic component is also perpendicular to the
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationIntroduction to XRay Powder Diffraction Data Analysis
Introduction to XRay Powder Diffraction Data Analysis Center for Materials Science and Engineering at MIT http://prism.mit.edu/xray An Xray diffraction pattern is a plot of the intensity of Xrays scattered
More informationUW Department of Chemistry Lab Lectures Online
Lab 5: Periodic Trends Part I: (Prelab) A Computer Study and Introduction to ChemDraw Part II: AcidBase Properties of Period 3 and Group 5A Elemental Oxides Part III: Oxidizing Ability of the Elemental
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationExplain the ionic bonds, covalent bonds and metallic bonds and give one example for each type of bonds.
Problem 1 Explain the ionic bonds, covalent bonds and metallic bonds and give one example for each type of bonds. Ionic Bonds Two neutral atoms close to each can undergo an ionization process in order
More informationCHEM 10113, Quiz 7 December 7, 2011
CHEM 10113, Quiz 7 December 7, 2011 Name (please print) All equations must be balanced and show phases for full credit. Significant figures count, show charges as appropriate, and please box your answers!
More informationTheory of XRay Diffraction. Kingshuk Majumdar
Theory of XRay Diffraction Kingshuk Majumdar Contents Introduction to XRays Crystal Structures: Introduction to Lattices Different types of lattices Reciprocal Lattice Index Planes XRay Diffraction:
More informationXray thinfilm measurement techniques
Technical articles Xray thinfilm measurement techniques II. Outofplane diffraction measurements Toru Mitsunaga* 1. Introduction A thinfilm sample is twodimensionally formed on the surface of a substrate,
More informationEach grain is a single crystal with a specific orientation. Imperfections
Crystal Structure / Imperfections Almost all materials crystallize when they solidify; i.e., the atoms are arranged in an ordered, repeating, 3dimensional pattern. These structures are called crystals
More informationLMB Crystallography Course, 2013. Crystals, Symmetry and Space Groups Andrew Leslie
LMB Crystallography Course, 2013 Crystals, Symmetry and Space Groups Andrew Leslie Many of the slides were kindly provided by Erhard Hohenester (Imperial College), several other illustrations are from
More information12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Crystal Geometry
12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Bibliography: Crystal Geometry Assigned Reading: [Poirier, 1985]Chapter 2, 4. General References: [Kelly and Groves, 1970] Chapter 1. [Hirth
More informationSolid State Theory Physics 545
Solid State Theory Physics 545 CRYSTAL STRUCTURES Describing periodic structures Terminology Basic Structures Symmetry Operations Ionic crystals often have a definite habit which gives rise to particular
More informationemission of light from atoms discrete line spectra  energy levels, FranckHertz experiment
Introduction Until the early 20 th century physicists used to explain the phenomena in the physical world around them using theories such a mechanics, electromagnetism, thermodynamics and statistical physics
More informationXray Diffraction (XRD)
Xray Diffraction (XRD) 1.0 What is Xray Diffraction 2.0 Basics of Crystallography 3.0 Production of Xrays 4.0 Applications of XRD 5.0 Instrumental Sources of Error 6.0 Conclusions Bragg s Law n l =2dsinq
More informationAtomic Force Microscope and Magnetic Force Microscope Background Information
Atomic Force Microscope and Magnetic Force Microscope Background Information Lego Building Instructions There are several places to find the building instructions for building the Lego models of atomic
More informationChapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More informationCoordination and Pauling's Rules
Page 1 of 8 EENS 2110 Tulane University Mineralogy Prof. Stephen A. Nelson Coordination and Pauling's Rules This document last updated on 24Sep2013 The arrangement of atoms in a crystal structure not
More informationWe shall first regard the dense sphere packing model. 1.1. Draw a two dimensional pattern of dense packing spheres. Identify the twodimensional
Set 3: Task 1 and 2 considers many of the examples that are given in the compendium. Crystal structures derived from sphere packing models may be used to describe metals (see task 2), ionical compounds
More informationChapter 13 The Chemistry of Solids
Chapter 13 The Chemistry of Solids Jeffrey Mack California State University, Sacramento Metallic & Ionic Solids Crystal Lattices Regular 3D arrangements of equivalent LATTICE POINTS in space. Lattice
More informationSimple vs. True Calculating Empirical and Molecular Formulas
17 Calculating Empirical and Molecular Formulas OBJECTIVE Students will learn to calculate empirical and molecular formulas and practice applying logical problemsolving skills. LEVEL Chemistry NATIONAL
More informationXray diffraction techniques for thin films
Xray diffraction techniques for thin films Rigaku Corporation Application Laboratory Takayuki Konya 1 Today s contents (PM) Introduction Xray diffraction method OutofPlane InPlane Pole figure Reciprocal
More informationDay I: Crystals and XRay Diffraction
Macromolecular Structure Determination I Day I: Crystals and XRay Diffraction Tim Grüne Dept. of Structural Chemistry, University of Göttingen September 2010 http://shelx.uniac.gwdg.de tg@shelx.uniac.gwdg.de
More informationEXPERIMENT O6. Michelson Interferometer. Abstract. References. PreLab
EXPERIMENT O6 Michelson Interferometer Abstract A Michelson interferometer, constructed by the student, is used to measure the wavelength of HeNe laser light and the index of refraction of a flat transparent
More informationEXPERIMENT 4: Electron Configuration of elements
Material: laboratory display of the elements and a wall periodic table is required. Objective: To learn the use of periodic table for writing electron configuration of elements. INTRODUCTION Basic building
More informationPhase determination methods in macromolecular X ray Crystallography
Phase determination methods in macromolecular X ray Crystallography Importance of protein structure determination: Proteins are the life machinery and are very essential for the various functions in the
More informationInterference. Physics 102 Workshop #3. General Instructions
Interference Physics 102 Workshop #3 Name: Lab Partner(s): Instructor: Time of Workshop: General Instructions Workshop exercises are to be carried out in groups of three. One report per group is due by
More information0 Introduction to Data Analysis Using an Excel Spreadsheet
Experiment 0 Introduction to Data Analysis Using an Excel Spreadsheet I. Purpose The purpose of this introductory lab is to teach you a few basic things about how to use an EXCEL 2010 spreadsheet to do
More informationXRay Diffraction: A Comprehensive Explanation for Multipurpose Research
XRay Diffraction: A Comprehensive Explanation for Multipurpose Research Adree Khondker 1, Shakir Lakhani 2 1 Westdale S.S., Hamilton, ON, Canada 2 Upper Canada College, Toronto, ON, Canada Abstract: The
More informationModelling Compounds. 242 MHR Unit 2 Atoms, Elements, and Compounds
6.3 Figure 6.26 To build the Michael LeeChin Crystal at the Royal Ontario Museum, models were used at different stages to convey different types of information. Modelling Compounds The Michael LeeChin
More informationSimple vs. True. Simple vs. True. Calculating Empirical and Molecular Formulas
Calculating Empirical and Molecular Formulas Formula writing is a key component for success in chemistry. How do scientists really know what the true formula for a compound might be? In this lesson we
More informationCRYSTALLINE SOLIDS IN 3D
CRYSTALLINE SOLIDS IN 3D Andrew Baczewski PHY 491, October 7th, 2011 OVERVIEW First  are there any questions from the previous lecture? Today, we will answer the following questions: Why should we care
More informationTransition metals: halffilled and fullyfilled subshells have extra stability. d 5 s 1 d 10 s 1
Unusual electron configurations Transition metals: halffilled and fullyfilled subshells have extra stability. d 5 s 1 d 10 s 1 Examples: Cr and Cu Transition metal ions: s and d energy levels change
More informationAustin Peay State University Department of Chemistry Chem 1111. The Use of the Spectrophotometer and Beer's Law
Purpose To become familiar with using a spectrophotometer and gain an understanding of Beer s law and it s relationship to solution concentration. Introduction Scientists use many methods to determine
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationEXPERIMENT 4 The Periodic Table  Atoms and Elements
EXPERIMENT 4 The Periodic Table  Atoms and Elements INTRODUCTION Primary substances, called elements, build all the materials around you. There are more than 109 different elements known today. The elements
More informationAtoms, Ions and Molecules The Building Blocks of Matter
Atoms, Ions and Molecules The Building Blocks of Matter Chapter 2 1 Chapter Outline 2.1 The Rutherford Model of Atomic Structure 2.2 Nuclides and Their Symbols 2.3 Navigating the Periodic Table 2.4 The
More informationElectromagnetic Radiation
Activity 17 Electromagnetic Radiation Why? Electromagnetic radiation, which also is called light, is an amazing phenomenon. It carries energy and has characteristics of both particles and waves. We can
More informationAP Chemistry A. Allan Chapter 8 Notes  Bonding: General Concepts
AP Chemistry A. Allan Chapter 8 Notes  Bonding: General Concepts 8.1 Types of Chemical Bonds A. Ionic Bonding 1. Electrons are transferred 2. Metals react with nonmetals 3. Ions paired have lower energy
More informationb) What is the trend in melting point as one moves up the group in alkali metals? Explain.
Problem Set 2 Wed May 25, 2011 1. What is the rough trend in the number of oxidation states available to the elements (excluding the noble gases) as you move a) to the right and b) down the periodic table?
More informationChapters 2 and 6 in Waseda. Lesson 8 Lattice Planes and Directions. Suggested Reading
Analytical Methods for Materials Chapters 2 and 6 in Waseda Lesson 8 Lattice Planes and Directions Suggested Reading 192 Directions and Miller Indices Draw vector and define the tail as the origin. z Determine
More informationThe Mole. 6.022 x 10 23
The Mole 6.022 x 10 23 Background: atomic masses Look at the atomic masses on the periodic table. What do these represent? E.g. the atomic mass of Carbon is 12.01 (atomic # is 6) We know there are 6 protons
More informationLAUE DIFFRACTION INTRODUCTION CHARACTERISTICS X RAYS BREMSSTRAHLUNG
LAUE DIFFRACTION INTRODUCTION Xrays are electromagnetic radiations that originate outside the nucleus. There are two major processes for Xray production which are quite different and which lead to different
More informationFRICTION, WORK, AND THE INCLINED PLANE
FRICTION, WORK, AND THE INCLINED PLANE Objective: To measure the coefficient of static and inetic friction between a bloc and an inclined plane and to examine the relationship between the plane s angle
More informationSample Exercise 12.1 Calculating Packing Efficiency
Sample Exercise 12.1 Calculating Packing Efficiency It is not possible to pack spheres together without leaving some void spaces between the spheres. Packing efficiency is the fraction of space in a crystal
More informationXray Crystallography Lectures
Xray Crystallography Lectures 1. Biological imaging by Xray diffraction. An overview. 2. Crystals. Growth, physical properties and diffraction. 3. Working in reciprocal space. Xray intensity data collection
More informationXRAY DIFFRACTION PROCEDURES
XRAY DIFFRACTION PROCEDURES For Polycrystalline and Amorphous Materials HAROLD P. KLUG HEAD OF THE DEPARTMENT OF RESEARCH IN CHEMICAL PHYSICS LEROY E. ALEXANDER SENIOR FELLOW IN XRAY DIFFRACTION Mellon
More informationEXPERIMENT 11 UV/VIS Spectroscopy and Spectrophotometry: Spectrophotometric Analysis of Potassium Permanganate Solutions.
EXPERIMENT 11 UV/VIS Spectroscopy and Spectrophotometry: Spectrophotometric Analysis of Potassium Permanganate Solutions. Outcomes After completing this experiment, the student should be able to: 1. Prepare
More informationPHOTOELECTRIC EFFECT AND DUAL NATURE OF MATTER AND RADIATIONS
PHOTOELECTRIC EFFECT AND DUAL NATURE OF MATTER AND RADIATIONS 1. Photons 2. Photoelectric Effect 3. Experimental Setup to study Photoelectric Effect 4. Effect of Intensity, Frequency, Potential on P.E.
More informationChapter 3: Structure of Metals and Ceramics. Chapter 3: Structure of Metals and Ceramics. Learning Objective
Chapter 3: Structure of Metals and Ceramics Chapter 3: Structure of Metals and Ceramics Goals Define basic terms and give examples of each: Lattice Basis Atoms (Decorations or Motifs) Crystal Structure
More information6) How wide must a narrow slit be if the first diffraction minimum occurs at ±12 with laser light of 633 nm?
Test IV Name 1) In a single slit diffraction experiment, the width of the slit is 3.1 105 m and the distance from the slit to the screen is 2.2 m. If the beam of light of wavelength 600 nm passes through
More informationLaue lens for Nuclear Medicine
Laue lens for Nuclear Medicine PhD in Physics Gianfranco Paternò Ferrara, 611013 Supervisor: prof. Vincenzo Guidi Sensors and Semiconductors Lab, Department of Physics and Earth Science, University of
More informationChapter 5 Polar Coordinates; Vectors 5.1 Polar coordinates 1. Pole and polar axis
Chapter 5 Polar Coordinates; Vectors 5.1 Polar coordinates 1. Pole and polar axis 2. Polar coordinates A point P in a polar coordinate system is represented by an ordered pair of numbers (r, θ). If r >
More informationCHAPTER 13 THE PERIODIC TABLE
CHAPTER 13 THE PERIODIC TABLE OVERVIEW The periodic table is usually the first thing that comes to mind when thinking about the subject of chemistry. We have all heard about the periodic table from as
More informationPERIODIC TABLE OF GROUPS OF ELEMENTS Elements can be classified using two different schemes.
1 PERIODIC TABLE OF GROUPS OF ELEMENTS Elements can be classified using two different schemes. Metal Nonmetal Scheme (based on physical properties) Metals  most elements are metals  elements on left
More informationBelow is a very brief tutorial on the basic capabilities of Excel. Refer to the Excel help files for more information.
Excel Tutorial Below is a very brief tutorial on the basic capabilities of Excel. Refer to the Excel help files for more information. Working with Data Entering and Formatting Data Before entering data
More informationThe Reaction of Calcium Chloride with Carbonate Salts
The Reaction of Calcium Chloride with Carbonate Salts PRELAB ASSIGNMENT: Reading: Chapter 3 & Chapter 4, sections 13 in Brown, LeMay, Bursten, & Murphy. 1. What product(s) might be expected to form when
More informationChapter 3. Molecules, Compounds, and Chemical Composition
Chapter 3 Molecules, Compounds, and Chemical Composition Elements and Compounds Elements combine together to make an almost limitless number of compounds. The properties of the compound are totally different
More informationPaper 1 (7404/1): Inorganic and Physical Chemistry Mark scheme
AQA Qualifications AS Chemistry Paper (7404/): Inorganic and Physical Chemistry Mark scheme 7404 Specimen paper Version 0.6 MARK SCHEME AS Chemistry Specimen paper Section A 0. s 2 2s 2 2p 6 3s 2 3p 6
More informationSection 1.1. Introduction to R n
The Calculus of Functions of Several Variables Section. Introduction to R n Calculus is the study of functional relationships and how related quantities change with each other. In your first exposure to
More informationGroup Theory and Chemistry
Group Theory and Chemistry Outline: Raman and infrared spectroscopy Symmetry operations Point Groups and Schoenflies symbols Function space and matrix representation Reducible and irreducible representation
More informationElectrons in Atoms & Periodic Table Chapter 13 & 14 Assignment & Problem Set
Electrons in Atoms & Periodic Table Name WarmUps (Show your work for credit) Date 1. Date 2. Date 3. Date 4. Date 5. Date 6. Date 7. Date 8. Electrons in Atoms & Periodic Table 2 Study Guide: Things You
More informationFor example, estimate the population of the United States as 3 times 10⁸ and the
CCSS: Mathematics The Number System CCSS: Grade 8 8.NS.A. Know that there are numbers that are not rational, and approximate them by rational numbers. 8.NS.A.1. Understand informally that every number
More informationModern Atomic Theory
Reading: Ch. 9, sections 14 Ch. 7, sections 56 (lec) Ch. 7, sections 13 (lab) Modern Atomic Theory Homework: Chapter 9: 37*, 39*, 41 Chapter 7: 59, 61*, 63, 65 (lec.) Chapter 7: 39, 41, 43, 47 (lab)
More informationMath 215 HW #6 Solutions
Math 5 HW #6 Solutions Problem 34 Show that x y is orthogonal to x + y if and only if x = y Proof First, suppose x y is orthogonal to x + y Then since x, y = y, x In other words, = x y, x + y = (x y) T
More informationChapter 2: Crystal Structures and Symmetry
Chapter 2: Crystal Structures and Symmetry Laue, ravais December 28, 2001 Contents 1 Lattice Types and Symmetry 3 1.1 TwoDimensional Lattices................. 3 1.2 ThreeDimensional Lattices................
More informationUnit 5 Elements and their Properties
Unit 5 Elements and their Properties 1. In 1871, Russian chemist Mendeleev created the forerunner of the modern periodic table. 2. The elements in Mendeleev's table were arranged in order of increasing
More informationSH1009, Modern Fysik. XRay Diffraction Muhammad Yasir, Lway al Maeeni, Joakim Wahlström
SH1009, Modern Fysik XRay Diffraction Muhammad Yasir, Lway al Maeeni, Joakim Wahlström 24 th april, 2009 Introduction In this lab we study the xrays and their ability to penetrate materials. We also
More informationSUPPLEMENTARY MATERIAL
SUPPLEMENTARY MATERIAL (Student Instructions) Determination of the Formula of a Hydrate A Greener Approach Objectives To experimentally determine the formula of a hydrate salt. To learn to think in terms
More informationWaves  Transverse and Longitudinal Waves
Waves  Transverse and Longitudinal Waves wave may be defined as a periodic disturbance in a medium that carries energy from one point to another. ll waves require a source and a medium of propagation.
More informationFURTHER VECTORS (MEI)
Mathematics Revision Guides Further Vectors (MEI) (column notation) Page of MK HOME TUITION Mathematics Revision Guides Level: AS / A Level  MEI OCR MEI: C FURTHER VECTORS (MEI) Version : Date: 97 Mathematics
More informationHolography 1 HOLOGRAPHY
Holography 1 HOLOGRAPHY Introduction and Background The aesthetic appeal and commercial usefulness of holography are both related to the ability of a hologram to store a threedimensional image. Unlike
More informationSample Exercise 8.1 Magnitudes of Lattice Energies
Sample Exercise 8.1 Magnitudes of Lattice Energies Without consulting Table 8.2, arrange the ionic compounds NaF, CsI, and CaO in order of increasing lattice energy. Analyze From the formulas for three
More informationSection 9.5: Equations of Lines and Planes
Lines in 3D Space Section 9.5: Equations of Lines and Planes Practice HW from Stewart Textbook (not to hand in) p. 673 # 35 odd, 237 odd, 4, 47 Consider the line L through the point P = ( x, y, ) that
More informationAtoms, Molecules, Formulas, and Subatomic Particles
Introduction to Chemistry Chapter 5 1 Atoms, Molecules, Formulas, and Subatomic Particles The Atom: The smallest particle of an element that can exist and still have the properties of the element building
More informationChapter 8 How to Do Chemical Calculations
Chapter 8 How to Do Chemical Calculations Chemistry is both a qualitative and a quantitative science. In the laboratory, it is important to be able to measure quantities of chemical substances and, as
More informationANSWER KEY. Energy Levels, Electrons and IONIC Bonding It s all about the Give and Take!
ANSWER KEY Energy Levels, Electrons and IONIC Bonding It s all about the Give and Take! From American Chemical Society Middle School Chemistry Unit: Chapter 4 Content Statements: Distinguish the difference
More informationLINES AND PLANES IN R 3
LINES AND PLANES IN R 3 In this handout we will summarize the properties of the dot product and cross product and use them to present arious descriptions of lines and planes in three dimensional space.
More informationO6: The Diffraction Grating Spectrometer
2B30: PRACTICAL ASTROPHYSICS FORMAL REPORT: O6: The Diffraction Grating Spectrometer Adam Hill Lab partner: G. Evans Tutor: Dr. Peter Storey 1 Abstract The calibration of a diffraction grating spectrometer
More informationCHAPTER 6 Chemical Bonding
CHAPTER 6 Chemical Bonding SECTION 1 Introduction to Chemical Bonding OBJECTIVES 1. Define Chemical bond. 2. Explain why most atoms form chemical bonds. 3. Describe ionic and covalent bonding.. 4. Explain
More informationStudents will understand 1. use numerical bases and the laws of exponents
Grade 8 Expressions and Equations Essential Questions: 1. How do you use patterns to understand mathematics and model situations? 2. What is algebra? 3. How are the horizontal and vertical axes related?
More informationThe Mole Concept. The Mole. Masses of molecules
The Mole Concept Ron Robertson r2 c:\files\courses\111020\2010 final slides for web\mole concept.docx The Mole The mole is a unit of measurement equal to 6.022 x 10 23 things (to 4 sf) just like there
More informationAP Chemistry A. Allan Chapter 7 Notes  Atomic Structure and Periodicity
AP Chemistry A. Allan Chapter 7 Notes  Atomic Structure and Periodicity 7.1 Electromagnetic Radiation A. Types of EM Radiation (wavelengths in meters) 101 1010 108 4 to 7x107 104 101 10 10 4 gamma
More informationUnit 8: Chemical Reactions and Equations
1 Chemical Reactions Unit 8: Chemical Reactions and Equations What are chemical reactions and how do they occur? How are chemical reactions classified? How are products of chemical reactions predicted?
More informationXray Powder Diffraction Pattern Indexing for Pharmaceutical Applications
The published version of this manuscript may be found at the following webpage: http://www.pharmtech.com/pharmtech/peerreviewed+research/xraypowderdiffractionpatternindexingfor Phar/ArticleStandard/Article/detail/800851
More informationhypothesis of Louis de Broglie (1924): particles may have wavelike properties
Wave properties of particles hypothesis of Louis de Broglie (1924): particles may have wavelike properties note: it took almost 20 years after noting that waves have particle like properties that particles
More informationChapter 6 The Periodic Table
Chapter 6 The Periodic Table Organizing the Periodic Table In a grocery store, the products are grouped according to similar characteristics. With a logical classification system, finding and comparing
More information